- Nano Express
- Open Access
Integrated nanophotonic hubs based on ZnO-Tb(OH)3/SiO2 nanocomposites
Nanoscale Research Letters volume 6, Article number: 503 (2011)
Optical integration is essential for practical application, but it remains unexplored for nanoscale devices. A newly designed nanocomposite based on ZnO semiconductor nanowires and Tb(OH)3/SiO2 core/shell nanospheres has been synthesized and studied. The unique sea urchin-type morphology, bright and sharply visible emission bands of lanthanide, and large aspect ratio of ZnO crystalline nanotips make this novel composite an excellent signal receiver, waveguide, and emitter. The multifunctional composite of ZnO nanotips and Tb(OH)3/SiO2 nanoparticles therefore can serve as an integrated nanophotonics hub. Moreover, the composite of ZnO nanotips deposited on a Tb(OH)3/SiO2 photonic crystal can act as a directional light fountain, in which the confined radiation from Tb ions inside the photonic crystal can be well guided and escape through the ZnO nanotips. Therefore, the output emission arising from Tb ions is truly directional, and its intensity can be greatly enhanced. With highly enhanced lasing emissions in ZnO-Tb(OH)3/SiO2 as well as SnO2-Tb(OH)3/SiO2 nanocomposites, we demonstrate that our approach is extremely beneficial for the creation of low threshold and high-power nanolaser.
Semiconductive photonic nanostructures have attracted increasing attention for its many possible applications, such as laser, solar cell, biosensor, and photoelectric conversion [1–4]. Among all the semiconductor materials, zinc oxide is of great interest for photonic applications due to its wide bandgap (3.37 eV) and efficient emission . The optoelectronic properties of zinc oxide depend critically on its defect structure and rich morphologies. ZnO nanostructures have been made into diverse morphologies, such as nanoparticles, nanorods, nanowires, nanobelts, and nanotubes [6–9]. Of these, ZnO nanorods have received the greatest attention and have shown to be a good laser emitter, an electron emitter, and a photoelectric converter. Their excellent optical behaviors are due to the fact that ZnO cannot only be a good gain medium but also can present good confinements for both photons and electrons. Numerical calculations have concluded that ZnO nanorods provide high lateral photonic confinement and are excellent waveguides . Light intensity losses occur only at the end faces, and this makes longer nanorods higher Q resonators. In addition, nanostructures like ZnO nanorods coupled with photonic nanomaterials can lead to newer applications.
When another optical nanostructure is coupled with ZnO, the integrated optical phenomenon can be demonstrated. We would like to study the coupling of ZnO and the strong luminescent nanomaterials of lanthanide hydroxide. Due to the unique electronic, optical, and magnetic properties arising from the 4f electrons, lanthanide hydroxides are very attractive in various applications, including catalysts, laser materials, biolabels, and magnetic resonance imaging . Previously, lanthanide-doped nanoparticles have been fabricated mainly by ion implantation , sol-gel method , and sonochemical synthesis . Unfortunately, the obtained size is often not uniform. Recently, we reported a one-pot synthesis of monodispersed core/shell Tb(OH)3/SiO2 colloids . The Tb(OH)3/SiO2 colloidal particles self-assembled into a 3-D photonic crystals (PCs), giving a pronounced optical gap depending on the particle size. Many efforts have been made on applications of PCs, such as the resonators, sensors, and reflectors [16–18]. To expand more applications of Tb(OH)3/SiO2 with other materials and nanostructures, semiconductor nanowires were chosen because they can be used as waveguides when attached to other luminescent materials . Based on the monodispersed Tb(OH)3/SiO2 core/shell nanoparticles, we report a novel composite with ZnO nanotip on Tb(OH)3/SiO2 core/shell nanoparticle (ZnO-Tb(OH)3/SiO2), which can be used to manipulate the emissions from inside the PCs. Due to the confinement effect of PC, emissions can escape only from the nanotips of ZnO. We found that the light output can be greatly enhanced by two orders of magnitude. To optimize this effect, SnO2 nanowires were selected to show the enhanced lasing emission of Tb(OH)3/SiO2 PCs by growing them on Tb(OH)3/SiO2 PCs of 130 nm which can perform better lasing action at 380 nm. Therefore, these novel composites act like directional light fountains, i.e., the light confined underneath the surface of the photonic crystal can be extracted only through the specially designed semiconductor nanotips. We show that this unique property is very useful to create low threshold and high-power nanolasers.
Nanoparticles of Tb(OH)3 were encapsulated inside silica as core/shell structures with an outer diameter of 250 nm by a one-pot synthesis method reported in our previous paper . The monodispersed nanoparticles were self-assembled on glass or Si (100) substrate by a slow evaporation method, resulting in self-organized packing as photonic crystals. After coating with gold nanoparticles (20 mA, 20 s), Tb(OH)3/SiO2 nanoparticles were used as templates in a vapor-liquid-solid process to grow ZnO nanowires on the nanospheres. The mixed C/Zn powders were placed in an alumina boat, which was loaded in the center of a tube furnace. The gold-coated lanthanide nanosphere substrate was placed in the same boat but apart from the mixed powders for about 3 cm. Argon was then introduced into the system with a flow rate of 200 sccm as the carrier gas. Afterwards, the tube was heated to 980°C at a rate of 40°C/min. The reaction lasted about 60 min. After the furnace cooled down, white color products formed on the surface of the lanthanide nanosphere substrate. For SnO2 nanowire growth, the C/Zn powders were replaced with C/Sn powders then follow the above steps. Cathodoluminescence (CL) experiments were performed at room temperature with a scanning electron microscopy (JSM 6500, JEOL Ltd., Tokyo, Japan). Excitation spectra were gathered by a PMT detector with a CL system (Gatan instrument, MonoCL3, Gatan, Inc., Pleasanton, CA, USA).
Results and discussion
Fabrication of ZnO-Tb(OH)3/SiO2 composites
When the ZnO nanotips are grown on Tb(OH)3/SiO2 nanospheres, they possess a wurtzite structure with a longer length of 15 μm (Figure 1a). In contrast, ZnO rods grown on sapphire under the same growth conditions are generally less than 5 μm long [20, 21]. As ZnO nanotips were grown on Tb(OH)3/SiO2 nanospheres, it gradually transforms from a hexagonal to a conical shape (Figure 1b). The conical tip shape and the high aspect ratio (approximately 150) of nanotips are especially beneficial for field emission application. Generally, more than one ZnO nanotip can be grown on each nanosphere. For the aggregation of Tb(OH)3/SiO2 nanospheres, the composite of the ZnO nanotips and nanospheres appears like a sea urchin as shown in Figure 1c.
When a ZnO nanotip adheres to a Tb(OH)3/SiO2 nanosphere (Figure 2a), one can collect the emission of excited Tb(OH)3/SiO2 nanoparticles at the end of ZnO and vice versa. Due to the multiple transition bands of Tb3+ (5D3-7F6, 381 nm; 5D3-7F5, 416 nm; 5D3-7F4, 439 nm; 5D3-7F3, 460 nm; 5D4-7F6, 491 nm; and 5D4-7F5, 546 nm; 5D4-7F4, 591 nm)  and band edge (380 nm) and defect emissions (500 nm) of ZnO, the complex emissions of ZnO-Tb(OH)3/SiO2 are illustrated with single ZnO nanotip-Tb(OH)3/SiO2 and urchin-like composites. As shown in Figure 2a, when a ZnO nanotip was excited by an electron beam at 2.3 μm apart from the center of Tb ion, the emissions of ZnO at 380 and 500 nm were propagated through the rod and then excited Tb giving rise to the CL spectrum emissions at 414, 438, 460, and 546 nm (Figure 2b). During the secondary excitation process, the Tb ion acts as a signal receiver and an emitter. Furthermore, as a result of the resonance between the propagating emission of ZnO at 380 nm (λ) and the SiO2 cavity (n = 1.5) with a diameter of 250 nm (D), the emission wavelength of ZnO at 380 nm in Tb(OH)3/SiO2 nanoparticles become 253 nm, which coincides with the cavity length. Thus, light can resonate inside the nanoparticles, and the detected emission with a wavelength of 380 nm outside the nanoparticle is highly enhanced.
For an urchin-like ZnO-Tb(OH)3/SiO2 composite, several ZnO nanotips diverge from the center as shown in the inset of Figure 3. Because several emissions of Tb overlap with the luminescence of ZnO nanotips, the defect emission at 300 nm which originated only from the defect state of silica was chosen to present the optical propagation properties. The lifetime of SiO2 can be extended to several seconds, depending on the calcination process, thus the emission of SiO2 can be detected by CL mapping . For stand-alone ZnO nanowire, there is no emission at 300 nm, thus the detected emission at 300 nm is certainly propagated from Tb(OH)3/SiO2. As the Tb(OH)3/SiO2 sphere was excited, the emission can be propagated and detected along ZnO nanotips as shown in a monochromatic CL image taken at 300 nm (Figure 3). When excited, the emissions of Tb ion also can be dispatched from the pivot to the tips of ZnO. This behavior therefore proved that ZnO-Tb(OH)3/SiO2 can act as a light distributor/emitter, which enables the signal coming from the center to be distributed into the surrounding ZnO tips. In addition, it acts as an optical receiver, which is able to collect the light injected at the end of ZnO nanotips. As demonstrated above, these ZnO-Tb(OH)3/SiO2 nanocomposites can function as a waveguide, a receiver, an emitter, as well as a distributor. Therefore, the nanocomposite can serve as a multifunctional integrated nanophotonic hub, which serves as an efficient control for injected light.
Photonic bandgap and CL spectra of Tb(OH)3/SiO2 PCs
The top and lateral SEM images show assembled Tb(OH)3/SiO2 PCs (250 nm diameter) of about 20 to 25 layers (as shown in Figure 4a, b). As the nanospheres self-assembled into a face-centered cubic structure, it formed a stop band along the Γ to L direction which gives a sharp drop in the transmittance spectrum at around 550 nm (Figure 4c). For a single Tb(OH)3/SiO2 nanoparticle, the CL spectrum exhibits several bright emission bands of transitions from D levels to F levels at room temperature, ranging from 350 to 650 nm (Figure 4d, dotted) . The defect emission of silica at 300 nm was extremely weak in comparison to the luminescence of Tb ion. As the nanoparticles self-assembled, the stop band effect led to the modification of the emissions for the Tb ion embedded in the PCs so that most emission bands were quenched as shown by the solid curve in Figure 4d. Note that the solid curve has been enlarged by 25 times compared with that of the dotted line. As the luminescence of the Tb ions was suppressed, the defect emission of silica at 300 nm became more pronounced. For Tb(OH)3/SiO2 PCs, little emission could be detected in the well-packed region due to the optical trap of the stop band. However, a CL image shows that the confined emissions of the Tb ions can escape from the crack region and be detected along the crack defects (inset of Figure 5b).
As the electron beam with a spot size of 1 μm to approximately 2 μm in diameter was focused on the Tb(OH)3/SiO2 PCs surface, CL spectra showed broadened bands of intra-4f transitions under a small excitation current. As the current reached 5 × 10-8 A, two sharp peaks of the CL spectrum appeared at 543 and 551 nm (Figure 5a), possibly due to the Stark effect of stimulated emission . With increasing current, the two peaks are more resolved, and the corresponding intensity increases nonlinearly as shown in Figure 5b. The nonlinear relationship between CL intensity and excitation current revealed a threshold current of 5 × 10-8 A, indicating a stimulated emission behavior. PCs have been used as a lasing cavity to stimulate the confined emission inside . The low threshold may arise from the release of optical resonance between emissions near the stop band and the cavity of PCs.
Lasing action of rice paddy-like ZnO-Tb(OH)3/SiO2 PCs nanocomposites
After ZnO nanotips were grown on patterned Tb(OH)3/SiO2 PCs, they formed as rice paddy-like ZnO-Tb(OH)3/SiO2 PCs nanocomposites (inset of Figure 6). At least 40 times CL intensity was obtained in comparison to that of Tb(OH)3/SiO2 PCs (Figure 6a). Giant optical enhancement was found in ZnO-Tb(OH)3/SiO2 PCs that the previously diminished emission of PCs was enhanced through the ZnO nanotips. This enhancement demonstrated that in addition to defects, the confined emission of Tb ions can be released by propagating along ZnO nanotips. Under the circumstances, the ZnO nanotips act like a directional light fountain, in which the confined radiation inside PCs can escape from ZnO nanotips. In retrospection of the development of lasing mode or optical resonance, attention has been mostly focused on materials or structures. However, the purpose of the waveguide adapted lasing cavity is to reduce the loss of propagated emission in omnidirection and collimate light in a specific direction. As a result, the output emission intensity can be greatly enhanced. Similarly, once the lasing mode of the PCs is excited, the emission can be efficiently guided. To explore this intriguing possibility, Tb(OH)3/SiO2 PCs with a diameter of 130 nm were used to demonstrate the amplified laser action. Figure 6b shows emission spectra of Tb(OH)3/SiO2 PCs with and without SnO2 nanowires under the same excitation current of 8 × 10-9 A. After the SnO2 nanowires were grown on Tb(OH)3/SiO2 PCs, the peak intensity near 380 nm has risen up to 20 times, and the full width at half maximum (FWHM) is about 2 nm. The lasing peak at 380 nm away from the stop band at 330 nm is attributed to the band edge lasing operation . The inset of Figure 6b shows the dependence of emission intensity on exciting energy for the Tb(OH)3/SiO2 PCs with SnO2 nanowires. Without the aid of SnO2 nanowires, the threshold for laser emission of Tb(OH)3/SiO2 PCs is evaluated at 4 × 10-8 A based on the result shown in Figure 5b. However, after SnO2 nanowires were grown on Tb(OH)3/SiO2 PCs, the threshold is reduced to 5 × 10-9 A.
With the designed ZnO-Tb(OH)3/SiO2 nanocomposite, a multifunctional integrated nanophotonic hub has been created. We have shown that growing ultra tapered ZnO nanotips on Tb(OH)3/SiO2 PCs can yield good control of emission out of PCs, in which the radiation confined underneath the PC surface can be well guided by the attached ZnO nanotips and escape from a designed direction. Similarly, SnO2 nanowires act as a directional light fountain, which may be very useful for the creation of ultra low threshold and high-power nanolaser. In view of the novel properties discovered here, the semiconductor Tb(OH)3/SiO2 composites pave a new way for the realization of applications of nanophotonics.
scanning electron microscopy
Chu KC, Su WS, Chen YF: Liquid crystals driven by CdSe semiconductors. J Appl Phys 2006, 100: 024516. 10.1063/1.2219697
Jiang Y, Zhang WJ, Jie JS, Meng XM, Zapien JA, Lee ST: Homoepitaxial growth and lasing properties of ZnS nanowire and nanoribbon arrays. Adv Mater 2006, 18: 1527–1532. 10.1002/adma.200501913
Liu C, Zapien JA, Yao Y, Meng XM, Lee CS, Fan SS, Lifshitz Y, Lee ST: High-density, ordered ultraviolet light-emitting ZnO nanowire arrays. Adv Mater 2003, 15: 838–841. 10.1002/adma.200304430
Gur I, Fromer NA, Chen CP, Kanaras AG, Alivisatos AP: Hybrid solar cells with prescribed nanoscaled morphologies based on hyperbranched semiconductor nanocrystals. Nano Lett 2007, 7: 409–414. 10.1021/nl062660t
Lin HY, Cheng CL, Chou YY, Huang LL, Chen YF: Enhancement of band gap emission by defect loss. Opt Exp 2006, 14: 2372–2379. 10.1364/OE.14.002372
Lin JM, Cheng CL, Lin HY, Chen YF: Giant enhancement of band edge emission in ZnO and SnO nanocomposites. Opt Lett 2006, 31: 3173–3175. 10.1364/OL.31.003173
Lin JM, Lin HY, Cheng CL, Chen YF: Giant enhancement of bandgap emission of ZnO nanorods by platinum nanoparticles. Nanotechnology 2006, 17: 4391–4394. 10.1088/0957-4484/17/17/017
Yang P, Yan H, Mao S, Russo R, Johnson J, Saykally R, Morris N, Pham J, He R, Choi HJ: Controlled growth of ZnO nanowires and their optical properties. Adv Func Mater 2002, 12: 323–331. 10.1002/1616-3028(20020517)12:5<323::AID-ADFM323>3.0.CO;2-G
Guo L, Yang S, Yang C, Yu P, Wang J, Ge W, Wong GKL: Highly monodisperse polymer-capped ZnO nanoparticles: preparation and optical properties. Appl Phys Lett 2000, 76: 2901–2903. 10.1063/1.126511
Hauschild R, Kalt H: Guided modes in ZnO nanorods. Appl Phys Lett 2006, 89: 123107. 10.1063/1.2354427
Mass H, Currao A, Calzaferri G: Encapsulated lanthanides as luminescent materials. Angew Chem Int Ed 2002, 41: 2495–2497. 10.1002/1521-3773(20020715)41:14<2495::AID-ANIE2495>3.0.CO;2-G
Slooff LH, Dood MJA, Blaaderen A, Polman A: Erbium-implanted silica colloids with 80% luminescence quantum efficiency. Appl Phys Lett 2000, 76: 3682–3684. 10.1063/1.126748
Zhao D, Qin W, Zhang J, Wu C, Qin G, De G, Zhang J, Lü S: Modified spontaneous emission of europium complex nanoclusters embedded in colloidal silica spheres. Chem Phys Lett 2005, 403: 129–134. 10.1016/j.cplett.2004.12.113
Patra A, Sominska E, Ramesh S, Koltypin Y, Zhong Z, Minti H, Reisfeld R, Gedanken A: Sonochemical preparation and characterization of Eu 2 O 3 and Tb 2 O 3 doped in and coated on silica and alumina nanoparticles. J Phys Chem B 1999, 103: 3361–3365. 10.1021/jp984766l
Lin YS, Hung Y, Lin HY, Tseng YH, Chen YF, Mou CY: Photonic crystals from monodisperse lanthanide-hydroxide-at-silica core/shell colloidal spheres. Adv Mater 2007, 19: 577–580. 10.1002/adma.200601371
Skorobogatiy M, Kabashin AV: Photon crystal waveguide-based surface plasmon resonance biosensor. Appl Phys Lett 2006, 89: 143518. 10.1063/1.2360186
Scharrer M, Yamilov A, Wu X, Hui C, Chang RPH: Ultraviolet lasing in high-order bands of three-dimensional ZnO photonic crystals. Appl Phys Lett 2006, 88: 201103. 10.1063/1.2203939
Kim TK, Yang SS, Son JK, Hong YG, Yang GM: GaN microcavity structure with dielectric distributed Bragg reflectors fabricated by using a wet-chemical etching of a (111) Si substrate. Appl Phys Lett 2006, 89: 041129. 10.1063/1.2236223
Pauzauskie PJ, Yang P: Nanowire photonics. Mater Today 2006, 9: 36–45.
Wang ZL: Nanostructures of zinc oxide. Mater Today 2004, 7: 26–33.
Baxter JB, Wu F, Aydil ES: Growth mechanism and characterization of zinc oxide hexagonal columns. Appl Phys Lett 2003, 83: 3797–3799. 10.1063/1.1624467
Soriano RB, Kpatcha E, Jakob AM, Merkert JW, Carlin CM, Schmedakea TA: Long-lifetime emission in luminescent colloidal silica. Appl Phys Lett 2007, 91: 091909. 10.1063/1.2771372
Amekura H, Eckau A, Carius R, Buchal C: Room-temperature photoluminescence from Tb ions implanted in SiO 2 on Si. J Appl Phys 1998, 84: 3867–3871. 10.1063/1.368591
Masuda H, Yamada M, Matsumoto F, Yokoyama S, Mashiko S, Nakao M, Nishio K: Lasing from two-dimensional photonic crystals using anodic porous alumina. Adv Mater 2006, 18: 213–216. 10.1002/adma.200401940
This work was supported by National Science Council of the Republic of China.
The authors declare that they have no competing interests.
HYL designed the structure and did the SEM, CL, and PL measurements. CLC carried out the ZnO growth and XRD characteristics. YSL and YH synthesized Tb(OH)3 nanoparticles and assembled them. CYM and YFC participated in the structure design and application. All authors read and approved the final manuscript.
Authors’ original submitted files for images
About this article
Cite this article
Lin, H.Y., Cheng, C.L., Lin, Y.S. et al. Integrated nanophotonic hubs based on ZnO-Tb(OH)3/SiO2 nanocomposites. Nanoscale Res Lett 6, 503 (2011) doi:10.1186/1556-276X-6-503